BIOMEDICAL REPORTS 4: 507-511, 2016
Antibacterial effect and shear bond strength of an orthodontic adhesive cement containing Galla chinensis extract LU‑FEI WANG1, FENG LUO1, CHAO‑RAN XUE1, MENG DENG2, CHEN CHEN1 and HAO WU3 1
State Key Laboratory of Oral Diseases, West China Hospital of Stomatology, Sichuan University, Chengdu 610072, P.R. China; 2 School of Dentistry, University of North Carolina at Chapel Hill, Chapel Hill, NC 27516, USA; 3Oral Department, Sichuan Academy of Medical Sciences and Sichuan Provincial People's Hospital, Chengdu 610072, P.R. China Received July 27, 2015; Accepted February 3, 2016 DOI: 10.3892/br.2016.603
Abstract. Galla chinensis extract (GCE), a naturally‑derived agent, has a significant inhibitory effect on cariogenic bacteria. The present study aims to evaluate the antibacterial effect and shear bond strength of an orthodontic adhesive cement containing GCE. A resin‑modified glass ionomer cement incorporated GCE at five mass fractions (0, 0.1, 0.2, 0.4, and 0.8%) to prepare GCE‑containing cement for analysis. For the agar diffusion test, cement specimens were placed on agar disk inoculated with Streptococcus mutans (strain ATCC 25175). Following 48 h incubation, the inhibition halo diameter was measured. To assess bacteria colonization susceptibility, S. mutans adhesion to cement specimens was detected by scanning electron microscopy (SEM) following 48 h incubation. To evaluate bond strength, a total of 50 metal brackets were bonded on premolar surfaces by using cement (10 teeth/group). Following immersion in an artificial saliva for 3 days, shear bond strength (SBS) was measured. The results demonstrated that GCE‑containing samples exhibited a larger bacterial inhibition halo than control, and the inhibition zone increased as the GCE mass fraction increased. SEM analysis demonstrated that S. mutans presented a weaker adherent capacity to all GCE‑containing cements compared with control, but the difference between each GCE‑containing group was not significant. SBS values of each GCE‑containing group exhibited no difference compared with the control. In conclusion, GCE‑containing adhesive cement exhibits a promising inhibitory effect on S. mutans growth and adhesion. Without compromising bond strength, adding GCE in adhesive cement may be an attractive option for preventing white spot lesions during orthodontic treatment.
Correspondence to: Dr Hao Wu, Oral Department, Sichuan Academy of Medical Sciences and Sichuan Provincial People's Hospital, No. 32 West Second Section First Ring Road, Chengdu 610072, P.R. China E‑mail: [email protected]
Key words: white spot lesions, Galla chinensis extract, adhesive cement, antibacterial effect, bond strength
Introduction The process of enamel demineralization and the development of white spot lesions around orthodontic brackets, fixed during orthodontic treatment constitutes a serious health issue, with a morbidity rate of ≤95% (1,2). The bonding of orthodontic brackets on the enamel surface can promote dental plaque accumulation, which results in the increased level of cariogenic bacteria, particularly Streptococcus mutans. Demineralization occurs when bacteria metabolize carbohydrates and produce organic acids, dissolving the calcium phosphate mineral of tooth structures (3). Cavitated lesions then develop if no effective therapeutic option is used (4). As the incidence of white spot lesions is increased following orthodontic treatment (1,5), the development of an effective preventive strategy against enamel demineralization around orthodontic brackets is necessary. Novel orthodontic bonding systems with antibacterial properties would be a promising strategy for preventing enamel demineralization, as cariogenic bacteria colonization and proliferation are the primary pathogenesis of white spot lesions (6‑8). Previous research has focused on developing novel antibacterial agents for improving orthodontic bonding systems, for example, fluoride, nano‑silver, titanium oxide, chlorhexidine and quaternary ammonium (9‑11). The use of substances derived from natural products has been extremely successful in the discovery of novel medicines (12). Galla chinensis, a traditional Chinese medicine, received much attention in the search of new bioactive agents for anti‑caries. The bioactive components of Galla chinensis extract (GCE) can suppress the growth of microcosm biofilms and inhibit lactic acid production (13). Furthermore, previous studies have demonstrated that GCE not only has a significant inhibitory effect on enamel demineralization (14), but also effectively promotes the remineralization of initial enamel carious lesion (15‑17). Furthermore, GCE seems to be the only natural product with the potential to regulate the balance of enamel demineralization/remineralization (18). We hypothesized that GCE could be a useful resource for developing an orthodontic bonding system with antibacterial properties. Therefore, the present study aimed to prepare a GCE‑containing adhesive cement for orthodontic use, and to evaluate its antibacterial effects and bonding strength.
WANG et al: GCE-CONTAINING ANTIBACTERIAL ADHESIVE CEMENT
Materials and methods Preparation of GCE‑containing cement. GCE was distilled as described previously (19). Briefly, Galla chinensis produced in Sichuan province, China was dried at 60˚C for 3 days, powdered, double extracted with distilled water, and then dissolved in ethanol for filtration and evaporation. Subsequently, the GCE was further fractionated by adsorption chromatography and purified by successive column chromatography. The obtained GCE was dissolved in ethanol and adjusted to pH 5.5. The GCE was incorporated into the liquid of resin‑modified glass ionomer cement (GC Fuji ORTHO™ LC, GC Corp., Tokyo, Japan) at certain mass fractions, which were pre‑set to ensure the mass fraction of GCE in cement mixture (following mixing of the liquid with powder). These values were 0 (control group), 0.1, 0.2, 0.4, and 0.8% respectively. Once the GCE‑containing cement sample was required for use, the cement liquid was mixed with the powder at a constant ratio, according to the manufacturer's instructions. Following this, 20 sec of LED light curing was performed (Ortholux, 3 M Unitek, Monrovia, CA, USA) for complete polymerization of the cement. Bacterial suspensions. As one of the most important cariogenic bacteria, S. mutans (strain 25175; American Type Culture Collection, Manassas, VA, USA) was selected for testing the antimicrobial properties of the GCE‑containing cement. The bacterial cells were cultured in Brain Heart Infusion (BHI) broth (BD Diagnostics, Franklin Lakes, NJ, USA) and incubated at 37˚C in a jar with a microaerophilic atmosphere enriched with 5% CO2 (Oxoid Campygen, Basingstoke, UK) until reaching the initial stationary phase after 48 h (Optical density at 650 nm of 0.30), and then measured using a Spectronic 20 (Milton Roy, Houston, TX, USA). The microbial suspension was used to inoculate the agar diffusion test plates and to perform the adhesion assay. Agar diffusion test. An agar diffusion test was adapted to evaluate antibacterial activity. S. mutans suspensions were inoculated on three plates with 20 ml of BHI agar. Five blocks were loaded on each plate and respective cement was introduced and light‑polymerized immediately. The plates were then incubated at 37˚C for 48 h, followed by the measurement of the inhibition halo diameters using a manual caliper. This was repeated three times, and mean values used for analysis. Bacteria colonization susceptibility. Six tubes containing 0.5 ml of S. mutans suspension were prepared. Cements with five mass fractions as described above, were photopolymerized into blocks respectively and then cut in 1‑2 mm size solid cubic particles with a scalpel blade. Three solid particles of each cement were placed in respective tubes in order to evaluate bacteria adhesion to cement specimens. A tube containing a pasteurized inactivated bacterial suspension was used as the negative control, in order to evaluate nonspecific adherence of the microorganism. The tubes were then incubated at 37˚C for 48 h in an atmosphere enriched with 5% CO2. Next, in order to remove not firmly adhered bacteria, all particles were washed three times in sterile culture medium and agitated for 10 sec at 1,400 rpm using an SA8 vortex mixer (Bibby Scientific Ltd., Stone, UK). The
Figure 1. Antibacterial activity of GCE‑containing cement in agar diffusion test. GCE‑containing samples exhibited larger bacterial inhibition halo than control, and inhibition zone increased as GCE mass fractions increased. Each value is mean ± SD. Bars with letters indicating values that are significantly different (P